Statement of problem
The marginal gap and ceramic bond strength of metal-ceramic restorations are important for success. However, studies evaluating the marginal gap and ceramic bond strength of fixed partial dentures (FPDs) produced with 3D printing technologies such as selective laser melting (SLM) are scarce.
The purpose of this in vitro study was to investigate the marginal gap of cobalt-chromium (Co-Cr) alloy frameworks produced by SLM technology before and after ceramic firing. Additionally, the metal-ceramic bond strength was evaluated with the Schwickerath crack-initiation test according to the International Standards Organization (ISO) 9693-1:2012.
Material and methods
Conventional impressions were made, and the definitive cast of a patient requiring a 4-unit FPD was scanned. After designing the FPD, the files were sent to a service center for the fabrication of a metal master model, 80 Co-Cr frameworks, and 80 flat specimens (25×3×0.5 mm) with SLM technology. The marginal gap between frameworks and the abutment tooth of the metal master model was nondestructively measured by using an optical coordinate-measuring machine. A total of 80 sets, consisting of 1 framework and 1 flat specimen, were sent to 80 dental laboratory technicians for ceramic firing. Detailed instructions for correct manipulation of the framework and flat specimen were provided. The marginal gap was remeasured, and the 3-point bend test was used to evaluate metal-ceramic bond strength.
Only 28 of the 80 dental technicians returned the specimens within a prespecified time and/or in adequate condition. The mean ±standard deviation marginal gap of the framework before ceramic firing was 25 ±9 μm and 34 ±12 μm after firing. The difference was statistically significant (P=.001). The mean ±standard deviation 3-point bend strength was 33 ±9 MPa.
Ceramic firing affected the marginal gap; however, all Co-Cr frameworks had a marginal gap lower than 120 μm, which is reported to be a clinically acceptable limit. Most of the specimens (80%) had a metal-ceramic bond strength value higher than the 25-MPa ISO 9693 requirement. Five of 28 dental laboratory technicians were not able to comply with ceramic firing instructions.
To read this article in full you will need to make a payment
Purchase one-time access:Academic & Personal: 24 hour online accessCorporate R&D Professionals: 24 hour online access
One-time access price info
- For academic or personal research use, select 'Academic and Personal'
- For corporate R&D use, select 'Corporate R&D Professionals'
Subscribe:Subscribe to Journal of Prosthetic Dentistry
Already a print subscriber? Claim online access
Already an online subscriber? Sign in
Register: Create an account
Institutional Access: Sign in to ScienceDirect
- Shear bond strength of a ceramic to Co-Cr alloys.J Prosthet Dent. 2008; 99: 54-59
- Effect of crown margins on periodontal conditions in regularly attending patients.J Prosthet Dent. 1991; 65: 75-79
- Effect of in vivo crown margin discrepancies on periodontal health.J Prosthet Dent. 1991; 65: 357-364
- The estimation of cement film thickness by an in vivo technique.Br Dent J. 1971; 131: 107-111
- The fit of cobalt-chromium three unit fixed dental prostheses fabricated with four different techniques: a comparative in vitro study.Dent Mater. 2011; 27: 356-363
- In vitro evaluation of marginal, axial, and occlusal discrepancies in metal ceramic restorations produced with new technologies.J Prosthet Dent. 2016; 116: 368-374
- Comparison of fatigue resistance and failure modes between metal-ceramic and all-ceramic crowns by cyclic loading in water.J Dent. 2014; 42: 1613-1620
- Shear bond strength of porcelain to a new millable alloy and a conventional castable alloy.J Prosthet Dent. 2015; 113: 329-335
- Computer-assisted milling of dental restorations using a new CAD/CAM data acquisition system.J Prosthet Dent. 1998; 80: 346-353
- Influence of porcelain firing and cementation on the marginal adaptation of metal-ceramic restorations prepared by different methods.J Prosthet Dent. 2017; 117: 656-661
- The precision of fit of cast and milled full-arch implant-supported restorations.Int J Oral Maxillofac Implants. 2013; 28: 687-693
- Evaluation of the fit of metal ceramic restorations fabricated with a pre-sintered soft alloy.J Prosthet Dent. 2016; 116: 916-923
- Clinical marginal and internal adaptation of CAD/CAM milling, laser sintering, and cast metal ceramic crowns.J Prosthet Dent. 2014; 112: 909-913
- In vitro assessment of the accuracy of digital impressions prepared using a single system for full-arch restorations on implants.Int J Comput Assist Radiol Surg. 2018; 13: 1097-1108
- The evolution of rapid prototyping in dentistry: a review.Rapid Prototyping J. 2009; 15: 216-225
- Selective laser melting technique of Co-Cr dental alloys: a review of structure and properties and comparative analysis with other available techniques.J Prosthodont. 2015; 24: 303-312
- Marginal fit changes during porcelain cycles.J Prosthet Dent. 1995; 73: 49-54
- Influence of finish line design on marginal adaptation of electroformed metal-ceramic crowns.J Prosthet Dent. 2006; 95: 237-242
- The effect of multiple firings on the marginal integrity of pressable ceramic single crowns.J Prosthet Dent. 2012; 107: 17-23
- Stress-relieving and porcelain firing cycle influence on marginal fit of commercially pure titanium and titanium-aluminum-vanadium copings.Dent Mater. 2003; 19: 686-691
- Effect of multiple firing on the bond strength of selected matched porcelain-fused-to-metal combinations.J Prosthet Dent. 1990; 63: 627-629
- Fracture reasons in ceramic-fused-to-metal restorations.J Oral Rehabil. 2003; 30: 265-269
- Marginal accuracy of titanium copings fabricated by casting and CAD/CAM techniques.J Prosthet Dent. 2006; 96: 47-52
- Longevity of fixed partial dentures.J Prosthet Dent. 1997; 78: 127-131
- Effects of repeated firing on the marginal accuracy of Co-Cr copings fabricated by selective laser melting.J Prosthet Dent. 2015; 113: 135-139
- In vitro precision of fit of computer-aided designed and computer-aided manufactured titanium screw-retained fixed dental prostheses before and after ceramic veneering.Clin Oral Implants Res. 2015; 26: 44-49
- A microcomputed tomography evaluation of the marginal fit of cobalt-chromium alloy copings fabricated by new manufacturing techniques and alloy systems.J Prosthet Dent. 2017; 117: 393-399
- Clinical marginal and internal fit of metal ceramic crowns fabricated with a selective laser melting technology.J Prosthet Dent. 2015; 113: 623-627
- Bond strengths of porcelain to cobalt-chromium alloys made by casting, milling, and selective laser melting.J Prosthet Dent. 2017; 118: 69-75
- Evaluation of metal-ceramic bond characteristics of three dental Co-Cr alloys prepared with different fabrication techniques.J Prosthet Dent. 2016; 116: 916-923
- Evaluation of the mechanical properties and porcelain bond strength of cobalt-chromium dental alloy fabricated by selective laser melting.J Prosthet Dent. 2014; 111: 51-55
- Comparison of porcelain bond strength of different metal frameworks prepared by using conventional and recently introduced fabrication methods.J Prosthet Dent. 2017; 118: 76-82
- Effects of multiple firings on metal-ceramic bond strength of Co-Cr alloy fabricated by selective laser melting.J Prosthet Dent. 2016; 115: 109-114
- Dentistry compability testing. Part 1: Metal-ceramic systems.International Organization for Standardization, Geneva2012 (ISO Store Order: OP-184149 (Date: 2017-06-09). Available at:)
- In vitro implant impression accuracy using a new photopolymerizing SDR splinting material.Clin Implant Dent Relat Res. 2015; 17: 721-729
- Optical properties of spectacle lenses computed by surfaces differential quantities.Adv Sci Lett. 2013; 19: 595-600
- On a criterion for the rejection of observations and the distribution of the ratio of deviation to sample standard deviation.Ann Math Stat. 1935; 6: 214-219
Published online: November 12, 2019
© 2019 by the Editorial Council for The Journal of Prosthetic Dentistry.